RESEARCH AND EDUCATION
Inﬂuence of denture tooth thickness on fracture mode of thin acrylic resin bases: An experimental and ﬁnite element analysis Takashi Sekinishi, DDS,a Shusuke Inukai, DDS, PhD,b Natsuko Murakami, DDS, PhD,b and Noriyuki Wakabayashi, DDS, PhDc The fracture resistance of acrylic ABSTRACT resin denture base is one of Statement of problem. The optimum selection of denture teeth for patients with a reduced the factors controlling the safety interarch distance has not been established. and longevity of removable Purpose. The purpose of this in vitro study was to investigate the inﬂuence of denture tooth prostheses, as well as patient material and thickness on the fracture resistance of thin acrylic resin denture bases. satisfaction. Previous reports Material and methods. Acrylic resin (AC), composite resin (CO), or ceramic (CE) molar denture have shown that acrylic resin teeth were embedded in denture base blocks (2.0 mm thick). The distance from the central fossa to fractures occur in 57% to 64% the tooth base was 0.5, 1.0, 2.0, or 2.5 mm for AC and CO, and 1.0 mm for CE (n=7), with a total of all removable dental prosthickness of 2.5 mm for all specimens. Each specimen was placed on a 3-point ﬂexural setup with a thesis failures1,2; these fractures shorter (8 mm) or longer (12 mm) support span than the tooth width and vertically loaded. A ﬁnite typically initiate at sites suselement analysis was performed to assess the stress distributions. The effects of tooth thickness and ceptible to masticatory stress.3-5 support span were statistically tested with ANOVA, followed by the Tukey honestly signiﬁcant difference post hoc test (a= .05). According to previous studies, the site of stress concentration Results. With the shorter support, the mean fracture load was higher in CO than AC, regardless of in the denture base may dethe tooth thickness. Under the longer support, the mean fracture load with the CO decreased pend on the position of the signiﬁcantly as the tooth thickness increased, with increased maximum stress. Some CO tooth specimens of 2.0 mm or 2.5 mm thickness failed at the tooth-denture base interface at signiﬁcantly denture teeth and retainer, lower loads than those exhibited by tooth fractures. CE showed minor cracks before bulk fracture. denture movement, and the occlusal scheme.6-10 The stress Conclusions. Higher fracture resistance was indicated with CO; however, the resistance decreased as the thickness of the CO tooth increased. (J Prosthet Dent 2015;114:122-129) is often concentrated by the reduced interarch distance at the posterior edentulous ridge area that results from the reported to decrease the strength of the acrylic resin denwear of the remaining natural teeth and/or the extrusion of ture base substantially,16 and experimental studies have opposing teeth.11,12 The opposing dentition may be in close found that the monomer priming of denture teeth and proximity to the alveolar ridges of the edentulous area. The surface treatment of repair resin both affect strength.17,18 mechanical requirements of a denture base that is to be Other experimental studies indicate that the denture subjected to high stress under masticatory function must be tooth material and cuspal angulations of the embedded optimized.13-15 The presence of a denture tooth has been tooth affect the pressure transfer capability of the denture
Supported by a Grant-in-Aid (24592902 to N.W. and 24792064 to S.I.) from the Japan Society for Promotion of Science/MEXT. Presented at the 122nd Annual Meeting of the Japan Prosthodontic Society, the 80th Anniversary, Fukuoka, Japan, May 2013. a Clinical Resident, Removable Partial Prosthodontics, Division of Oral Health Sciences, Tokyo Medical and Dental University (TMDU), Tokyo, Japan. b Assistant Professor, Removable Partial Prosthodontics, Division of Oral Health Sciences, Graduate School, Tokyo Medical and Dental University (TMDU), Tokyo, Japan. c Professor, Removable Partial Prosthodontics, Division of Oral Health Sciences, Graduate School, Tokyo Medical and Dental University (TMDU), Tokyo, Japan.
THE JOURNAL OF PROSTHETIC DENTISTRY
Table 1. Denture tooth specimens
Clinical Implications This in vitro study suggests that in partially and completely edentulous patients with a reduced interarch distance, a composite resin denture tooth is indicated, and that the acrylic resin denture base layer underneath the tooth bottom should have a thickness of at least 1.0 mm. A ceramic tooth may be contraindicated for a thin denture base because of early chipping.
base under impact loading.19,20 Nevertheless, the selection of denture tooth material and thickness in patients with reduced interarch distance remains controversial, and recommendations have not yet been established. The purpose of this study was to investigate the inﬂuence of the denture tooth material and thickness on the fracture mode of a thin acrylic resin denture base. A single molar denture tooth embedded in a rectangular denture base block of acrylic resin was modeled for the loading experiment and ﬁnite element analysis. An analysis of fracture mechanisms is necessary before in vitro testing of material strength can be considered clinically valid. An understanding of the stress distribution in the denture base with an embedded tooth under loading may reveal the underlying fracture mechanism. The hypothesis was that the fracture mode and resistance of the thin acrylic resin denture base would depend on the material and thickness of the tooth. MATERIALS AND METHODS Specimen preparation Each specimen consisted of a mandibular ﬁrst molar denture tooth embedded in an acrylic resin denture base block. Commercial denture teeth of 3 different materials were used: acrylic resin (AC), composite resin (CO), and ceramic (CE) (Table 1). The base of the AC and CO teeth were ground so that the distance between the central fossa and tooth base was 0.5 mm, 1.0 mm, 2.0 mm, or 2.5 mm (Fig. 1). The same procedure was conducted for CE to obtain a distance of 1.0 mm. For each tooth material, a specimen replica was created by embedding 1 of the polished teeth into a wax block 20 mm long, 12 mm wide, and 2 mm thick.16 The tooth was placed in the block with the buccolingual surfaces parallel to the length of the block and the mesiodistal occlusal groove parallel to the center of the long axis. The vertical distance from the central fossa to the bottom of the wax block was standardized at 2.5 mm for all specimens. A mold for the replica was made with silicone impression material (Duplicone; Shofu). For each specimen, a polished denture tooth was placed in the mold, and molten wax (Inlay Wax Medium; GC Corp) poured. Each wax block with a Sekinishi et al
Manufacturer Code Mold Shade Lot No.
Acrylic resin Wearless Acrylic
tooth was invested (Advastone; GC Corp), the wax was removed, and a heat-polymerizing denture base material (Acron; GC Corp) was processed at 75 C for 8 hours. Each specimen was then recovered and ﬁnished with #600 abrasive paper (DCCS; Sankyo-Rikagaku) to obtain a 2-mm thick block. Seven specimens were made for each material, thickness, and support span combination.16 The sample size was determined based on the results of a preliminary study, in which a relatively low standard error was observed for one of the thicknesses used. Fracture test Each specimen was subjected to a ﬂexural test with axial loading units (Autograph AGS-H; Shimadzu). Each specimen was placed on 2 metal supports of a shorter (8 mm) or a longer (12 mm) span compared to the buccolingual tooth width (approximately 10 mm). A spherical wedge with a 2 mm radius engaged the central groove of each tooth during loading (Fig. 2). The CE specimens were tested by using the longer support. Each specimen was deﬂected with a vertical crosshead speed of 5 mm/ min until fracture occurred. The results were evaluated on a comparative basis with the statistical methods described subsequently and also by comparisons with the reported maximal occlusal force of normal individuals or denture wearers.21-24 After the load test, the fractured specimens were observed with optical light microscopy at ×25 magniﬁcation (AX70PROVIS; Olympus) to evaluate the fracture initiation site and fracture mode. Some specimens were coated with platinum, and the surface was observed by scanning electron microscopy (S-4500 SEM; Hitachi Ltd). Nanoindentation test To determine the material properties of the ﬁnite element model of the composite resin denture (CO) specimen, the elastic moduli and hardness of the CO tooth and the acrylic resin denture base materials were measured with a nanoindentation test (ENT-1100a; Elionix). The crosssectional material surfaces were ﬁne polished to a particle size of 0.06 mm with silicon carbide papers and aluminum oxide slurry. Like most composite resin denture teeth, the CO contains an acrylic resin layer in its lower portion to enhance its bonding capability to the acrylic resin denture base.25-27 Seven indentation points were arbitrarily selected for each of the denture base, enamel, dentin, and base layers of the CO. The Martens THE JOURNAL OF PROSTHETIC DENTISTRY
Volume 114 Issue 1
2.5 mm X
12 mm 8 mm 12 mm 20 mm Figure 1. Tested specimens and dimensions. Upper, seen from mesiodistal direction. Tooth thickness (X) was 0.5, 1.0, 2.0, or 2.5 mm. Lower, seen from above.
hardness and elastic modulus were then measured at a maximum force of 50 mN by using a Berkovich indenter attached to a nanoindentation device. The modulus was calculated in accordance with the following equation, based on the load-displacement curve: −1 Er= 1 ns2 Es+ 1 ni2 Ei ; where Er is the effective modulus from the nanoindenter, Es is the modulus of the specimen, Ei is the modulus of the indenter, ns is the Poisson ratio for the specimen, and ni is the Poisson ratio of the indenter. To avoid accumulating data from indentations performed on the hard ﬁllers rather than on the matrix, the shape of the indentation, the load-displacement curve, and the range of the hardness data were closely inspected.28 Table 2 shows the mean Martens hardness and elastic modulus of the CO tooth and the acrylic resin denture base material. Finite element analysis Three-dimensional ﬁnite element models of the 1.0 mm or 2.0 mm thick CO specimens with 2 support spans were constructed to simulate the loading test (Fig. 3). Each model consisted of approximately 170 000 hexahedral elements, as determined by preliminary convergence tests (ANSYS 11.0; ANSYS Inc).29 All materials were homogeneous, linearly elastic, and isotropic. The mean moduli obtained by the nanoindentation test were entered into the program. The interface between the side tooth surface and the block was assumed to be completely bonded or in contact with a 0.3 friction coefﬁcient. A 0.3 mm vertical displacement was applied at the loading contact. The maximum principal stress distributions in the block were analyzed. Statistical analysis Statistical software (SPSS v11.5J for Windows; IBM) was used to detect signiﬁcant differences in the maximum THE JOURNAL OF PROSTHETIC DENTISTRY
Figure 2. Three-point ﬂexural loading test. Two different support lengths, 8 mm or 12 mm support length.
Table 2. Martens hardness and elastic modulus of composite resin tooth and denture base resin Material Denture base resin
Martens Hardness (GPa), Mean (SD)
Elastic Modulus (GPa), Mean (SD)
Composite resin tooth Enamel layer
load between different tooth thicknesses and materials. The data stratiﬁed by specimen thickness were compared by 1-way ANOVA. The Tukey honestly signiﬁcant difference test was used for post hoc analysis when equal variances could not be assumed (a=.05). The Tamhane T2 test was used only for the CO specimens under the shorter support for post hoc analysis because equal variances could not be assumed (a=.05). In addition, the AC and CO specimens were each compared according to support length with 2-way ANOVA. RESULTS All the AC and CO specimens exhibited fractures that initiated at the bottom surface of the blocks. The fracture modes were classiﬁed into 3 groups as follows (Fig. 4): (1) center-to-tooth mode, in which an initial crack occurred at the center of the bottom surface of the block, followed by the tooth fracture; (2) edge-to-tooth mode, in which the crack occurred at the bottom surface right under the edge of the tooth, the crack subsequently propagating obliquely upward to the center of the occlusal surface; and (3) edge-to-edge mode, in which the crack occurred at the bottom surface right under the edge of the tooth, the crack subsequently propagating vertically upward without a tooth fracture. For all specimens tested on the shorter support, fractures occurred in the center-to-tooth mode. For the longer support, all specimens exhibited fractures in the center-to-tooth or edge-to-tooth modes, except for 9 AC specimens (two 2.0 mm thick and all 2.5 mm thick) Sekinishi et al
Figure 3. Finite element model descriptions and stress distributions of denture base block. A, Model components in cross-sectioned half views: (e) enamel; (d) dentin; (b) acrylic resin denture base block; and (s) metallic supports. B, Components assembled and meshed to create ﬁnite element model. Side surface of (e) was assumed to be bonded or contacted with denture base block (b) (light blue lines).
Figure 4. Fracture modes. Dashed line and rectangular area in schematic illustrations of each fracture mode indicate fracture line and the viewing area for optical microscopic image (original magniﬁcation, ×25). All representative images were obtained from CO specimens. A, Arrow indicates viewing angle. B, Center-to-tooth fracture mode. C, Edge-to-tooth fracture mode. D, Edge-to-edge fracture mode.
and 5 CO specimens (one 2.0 mm thick and four 2.5 mm thick) that were in the edge-to-edge mode. On the basis of the observations of specimens exhibiting the center-to-tooth mode, most AC specimens cracked at the interface between the side tooth surface and the block, but such cracks were not found in the CO specimens (Fig. 5). Sekinishi et al
With the shorter support, tooth thicknesses between 0.5 mm and 2.5 mm did not signiﬁcantly affect the maximum load on the AC and CO specimens (P>.05). However, the mean maximum load was signiﬁcantly higher in the CO than that in the AC (P.05). THE JOURNAL OF PROSTHETIC DENTISTRY
Volume 114 Issue 1
AC or CO
the edge-to-edge mode (without tooth fracture) had a signiﬁcantly lower maximum load than those of the other fracture modes (with tooth fracture) (P